Effect of cr doping in structure and magneto transport properties of (la0.67 sr0.33)mno3
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.19, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications130Effect of Cr doping in Structure and Magneto-transportProperties of (La0.67Sr0.33)MnO3Tejas M. Tank*, Deepshikha Bhargava, S. P. SanyalSolid State Physics Laboratory, Department of Physics, Barkatullah University, Bhopal – 462 026, India*E-mail: firstname.lastname@example.orgAbstractThe study of perovskite manganites La0.67Sr0.33Mn1-xCrxO3 (0≤ x ≥0.10) has been carried out. The structure andmagneto-transport properties of La0.67Sr0.33Mn1-xCrxO3 manganites are strongly dependent on the doping level x.Polycrystalline samples of La0.67Sr0.33Mn1-xCrxO3 (0≤ x ≥0.10) were prepared by solid state reaction method. Thelittle difference between the ionic radii of Cr3+and Mn3+causes no change in the structure, the structure remainsrhombohedral. The temperature dependence of the resistivity is measured from 5 – 400 K without and withmagnetic field upto 5 T. The value of metal-insulator (M-I) transition temperature (TP) decreases when resistivityincreases for all the samples while doping level x increases. The value of magnetoresistance (MR %) increaseswith increases Cr doping level for all samples. We have calculated energy band gap (Eg) for all samples and it isrevealed that as per doping level increases Eg increases which is comparable with experimental data. So, thestructure and magneto-transport behavior pretentious by Cr doping.Keywords: Colossal magnetoresistance, metal-insulator transition.PACS: 75.47.Gk; 71.30.+h;INTRODUCTIONThe physical properties of the hole doped manganites is one of the most studied topics in the last oneand half decade due to the observation of ‘‘colossal’’ magnetoresistance (CMR) . The basic magnetic andstructural properties of R1-xAxMnO3 (R: rare earth, A: Ca, Ba, Sr) were widely studied in the past. Both endmembers – LaMnO3 and AMnO3 – of La1-xAxMnO3 (A = Ca, Sr, Pb, Ba, etc) are antiferromagnetic insulators,but, doped compounds (0.2 < x < 0.4) exhibit metal-insulator transition in concomitant with the ferromagnetic-paramagnetic transition. The extraordinary electronic and magnetic properties of colossal magnetoresistance(CMR) materials R1−xAxMn1−yByO3 (where R is a trivalent rare earth and A is a divalent alkali earth, B istransition metal) have attracted considerable attention during the past decade. In these perovskite compounds,interplay between magnetism, charge ordering, and electronic transport have been studied in detail . Inmanganites Mn ions play a crucial role in shaping the magnetic properties. Effects of Mn site substitution withdifferent elements such as Fe, Ni, Co etc. on the TC and other physical properties have been reported by someworkers . We report here a thorough study on the effects of the replacement of Mn by Cr in the colossalmagnetoresistive La0.67Sr0.33MnO3. Replacing trivalent Cr ion with Mn ion provides us a system to understandweakened double-exchange (DE) interaction (Mn3+- O- Cr3+) and the effect of co-doping of electrons on thesystem with a network of Mn3+- O- Cr3+and Mn4+- O- Cr4+. In this paper, we report the results of structural andtransport properties and also energy band gap calculation on La0.67Sr0.33Mn1-xCrxO3 (0≤ x ≥0.10) compounds.This made it possible to determine change in the electrical transport near the metal- insulator transition in thiscompound.EXPERIMENTALPolycrystalline samples of La0.67Sr0.33MnO3 (LSMO), La0.67Sr0.33Mn0.95Cr0.05O3 (LSMCO-5) andLa0.67Sr0.33Mn0.90Cr0.10O3 (LSMCO-10) were synthesized by the solid state reaction method. Stoichiometricmixture of respective oxide powders was ground and reacted at 1100 ºC for 24 h in air. The samples werereground, pressed into pellets, heated again and sintered at 1300 ºC for 24 h. The structure and phase purity ofsamples were confirmed by Powder X-ray diffraction using Cu Kα radiation at room temperature. Thetemperature dependence of the resistivity was measured from 5 – 400 K without and with applied magnetic fieldupto 5 T. The magnetic field dependence magnetoresistance carried out at various temperatures.RESULTS AND DISCUSSIONFigure 1 shows the XRD patterns of La0.67Sr0.33Mn1-xCrxO3 with x=0, 0.05 and 0.10. The XRD analysisindicates that all samples are single phase with perovskite rhombohedral structure and lattice cell parameters andunit cell volume are tabulated in Table 1. No impurity phase is observed in the XRD patterns, which suggest thatthe doped Cr substitute mainly for Mn. The similarity between the crystal structures of pure and Cr-dopedsamples imply that the doped Cr3+ion does not change the crystalline structure of pure LSMO, which maymainly result from the similar ionic size of Mn3+and Cr3+and the structure remains rhombohedral.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.19, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications131TABLE 1. Lattice Parameters and Unit Cell Volume for La0.67Sr0.33Mn1-xCrxO3 samples.Sample Code Lattice Parameters ( Å ) Unit Cell Volume(Å)3a (Å) b (Å) c (Å)LSMO 5.4797 5.4797 13.4040 402.483LSMCO-5 5.4767 5.4767 13.3749 401.169LSMCO-10 5.4741 5.4741 13.3600 400.342FIGURE 1: X-ray diffraction patterns for La0.67Sr0.33Mn1-xCrxO3 with x=0, 0.05 and 0.10 samples.Figure 2 demonstrates the temperature dependence of resistivity under 0 T, 1 T, 3 T and 5 T magneticfields. When Mn is partly substituted by Cr, the system displays a complicated and interesting transport behavior.With increasing Cr content, the M–I transition near TP shifts to lower temperature; meanwhile an additionalbump grows up subsequent to it. The coexistence of two bumps of CMR results in CMR remains in a broadtemperature range from the lowest (T2) to above room temperature (T1). The double-peaked feature of ρ-T curvehas been also observed in high doping level (y ≥ 0.07) La0.67A0.33Mn1-yByO3 . In the absence of a magneticfield LSMCO shows Tmin in the vicinity of 60 K. Assorted possible causes for the low-temperature resistivityminimum in the LSMCO sample are considered. These include the grain boundary, phase-separation, andelectron-electron localization . To confirm these reasons, work is under process by using theoretical model.The value of metal-insulator (M-I) transition temperature (TP) decreases when resistivity increases for all thesamples while doping level x increases. The resistivity and TP are listed in Table-2.TABLE 2. Metal-Insulator Transition Temperature and Resistivity for La0.67Sr0.33Mn1-xCrxO3 samples.Sample Code M-I Transition (TP) K Resistivity (ρ) Ω*cmLSMO 373 0.0356LSMCO-5351 (T1)289 (T2)0.04500.0419LSMCO-10 327 (T1) 0.0548257 (T2) 0.0506
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.19, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications132FIGURE 2. Temperature dependence of resistivity of La0.67Sr0.33 Mn1-xCrxO3 with and without magnetic fields.Therefore, it should be ascribed to the crucial role of Cr. It suggests that Cr element substitution on Mnsite can be a potent way in tuning CMR response. This suggests that it originates from the same mechanismbased on the DE between Mn ions as in undoped La0.67Sr0.33MnO3. As we mentioned that, there is a possibility ofDE through Mn3+–O–Cr3+due to the identical electronic configuration between Cr3+and Mn4+. The presentresults of CMR behavior in La0.67Sr0.33Mn1-xCrxO3 could be supporting evidence to this view. We have calculatedenergy bandgap (Eg) of for all samples and it is revealed that as per doping level increases Eg increases which iscomparable with experimental data as well as due to the interruption of well known phenomena of exchangebetween Mn3+and Mn4+while as the magnetic field increases Eg decreases for each samples which istheoretically provide evidenced of CMR  and Eg values for each samples tabulated in Table 2. One can seethat Cr doping is inefficiency in lowering TP, which imply that there might exist FM interaction between Mn3+and Cr3+. Considering those electrical properties, we assume that a FM interaction between Cr3+and Mn3+issimilar to the traditional Mn3+-O-Mn4+DE process. Because of the different effect of the crystal field over Mn4+and Cr3+, this cause an energetic difference between eg orbital levels of Mn3+and Cr3+, which becomes strongenough to result in that electronic exchange between them that is not equivalent to that between Mn3+and Mn4+.Hence, the DE interaction between Mn3+and Cr3+is similar to the DE interaction between Mn3+and Mn4+but theformer is weaker than the latter.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.19, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications133FIGURE 3: The Temperature vs. MR % for La0.67Sr0.33Mn1-xCrxO3 at various magnetic fields.SampleMagnetoresistance1T 3T 5TMR% T (K) MR% T (K) MR% T (K)LSMOLSMCO-5LSMCO-108911371354327101213372353327171820372354327TABLE 3. Temperature dependent MR % at 1, 3 and 5 T magnetic fields for La0.67Sr0.33Mn1-xCrxO3 samples.The samples show a significant change in resistance with the applied magnetic field. In other words,they bear varying amount of MR. We show in Fig. 3, the variation of MR value with applied magnetic field atdifferent temperatures. It is clear from Fig. 3 that the prominent MR at very low temperature, the low-field (< 1T) MR for Cr doped samples of about 32 % may be attributed to the intergranular spin polarized tunneling (SPT)of carriers . Thus, it is noted that, at low temperatures, the grain boundary has a significant contribution to theelectrical resistivity of the bulk sample. This is usually observed in polycrystalline samples and may result fromthe grain boundary effect. MR value increases gradually with magnetic field for all samples.CONCLUSIONIn conclusion, Cr doping at Mn site weakened double-exchange interaction is reflected in theprogressive decrease in metal-insulator transition (TP) and transport and magneto transport properties inmanganite and FM interaction between Cr3+and Mn3+is similar to the traditional Mn3+-O-Mn4+DE process.ACKNOWLEDGEMENTSThe Authors are thankful to Dr. R. Rawat, Dr. V. Ganesan and Dr. M. Gupta of UGC-DAE CSR, Indore forhelp in experimental work and to UGC, New Delhi through the research project (No. F. No. 37-90/2009 (SR))and Special Assistance Programme (SAP). Tejas M. Tank would like to acknowledge UGC-SAP, New Delhi,India for award of UGC (SAP) – JRF.
Advances in Physics Theories and Applications www.iiste.orgISSN 2224-719X (Paper) ISSN 2225-0638 (Online)Vol.19, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications134REFERENCES1. C. N. R. Rao and B. Raveau, Colossal Magnetoresistance, Charge Ordering and Related Properties andManganese Oxides, first ed., World Scientific, Singapore (1998).2. N. Gayatri, A. K. Raychaudhuri, S. K. Tiwary, R. Gundakaram, A. Arulraj and C. N. R. Rao, Phys. Rev. B56, 1345 (1997).3. B Raveau, Phil. Trans. R. Society A 366, 83 (2008).4. N. Paunović, Z. V. Popović, A. Cantarero, F. Sapina, Science of Sintering 40, 55 (2008).5. B. L. Altshuler and A. G. Aronov, in Electron-Electron Interaction in Disordered Systems, edited by A. L.Efrosand M. Pollak, North Holland, Amsterdam (1985).6. M.F.Thorpe, Physics of Manganites, edited by T. Kalpan and S. Mahanti, New York (2002).7. H. Y. Hwang, S. W. Cheong and B. Batlogg, Phys. Rev. Letter 77, 2041 (1996).
This academic article was published by The International Institute for Science,Technology and Education (IISTE). The IISTE is a pioneer in the Open AccessPublishing service based in the U.S. and Europe. The aim of the institute isAccelerating Global Knowledge Sharing.More information about the publisher can be found in the IISTE’s homepage:http://www.iiste.orgCALL FOR PAPERSThe IISTE is currently hosting more than 30 peer-reviewed academic journals andcollaborating with academic institutions around the world. There’s no deadline forsubmission. Prospective authors of IISTE journals can find the submissioninstruction on the following page: http://www.iiste.org/Journals/The IISTE editorial team promises to the review and publish all the qualifiedsubmissions in a fast manner. All the journals articles are available online to thereaders all over the world without financial, legal, or technical barriers other thanthose inseparable from gaining access to the internet itself. Printed version of thejournals is also available upon request of readers and authors.IISTE Knowledge Sharing PartnersEBSCO, Index Copernicus, Ulrichs Periodicals Directory, JournalTOCS, PKP OpenArchives Harvester, Bielefeld Academic Search Engine, ElektronischeZeitschriftenbibliothek EZB, Open J-Gate, OCLC WorldCat, Universe DigtialLibrary , NewJour, Google Scholar